Viscoelasticity  Home  Scholars at Harvard .sPa) and glass (· ~ 1012 sPa). 2. ... Linear...
date post
29Aug2018Category
Documents
view
219download
0
Embed Size (px)
Transcript of Viscoelasticity  Home  Scholars at Harvard .sPa) and glass (· ~ 1012 sPa). 2. ... Linear...
ES240 Solid Mechanics Fall 2009
11/4/12 Linear Elasticity1
Viscoelasticity
References
N.G. McCrum, C.P. Buckley, and C.B. Bucknall, Principles of Polymer Engineering, 2nd edition, Oxford University Press, 1997. A good balance of theory and application for a first introduction.
John J. Aklonis and W.J. MacKnight, Introduction to Polymer Viscoelasticity. Wiley, New York, 1983.
J.D. Ferry, Viscoelastic properties of polymers. 3rd edition, Wiley, New York, 1980.
R.M. Christensen, Theory of Viscoelasticity, 2nd edition. Dover Publications, Inc. New York, 1982. This book describes many boundary value problems.
1. Newtons law of viscous deformation
Subject to a load, a liquid flows. The amount of deformation is timedependent and unlimited. When the load is removed, the liquid does not recover its original shape. The liquid has no memory.
To characterize such deformation, we subject the liquid to a state of shear stress , and then measure the shear strain as a function of time t. The record, ( )t , allows us to calculate the strain rate dtd / . For some liquids, we may be able to fit the experimental data to a linear relation between the strain rate and the stress. If we can, we write
ddt
=
.
This linear fit is known as Newtons law of viscous deformation. (Some peoples names simply stick whatever they do.) The fitting parameter, , is known as the viscosity of the liquid. The viscosity has the dimension of time stress, and is specific to each liquid; e.g., water ( ~ 103 sPa) and glass ( ~ 1012 sPa).
2. Arrhenius equation
For a given liquid, the viscosity decreases as the temperature increases. A liquid flows when molecules pass one another, a process that is thermally activated. Thus, the relation between the viscosity and the temperature is often fit to the Arrhenius equation
ES240 Solid Mechanics Fall 2009
11/4/12 Linear Elasticity2
= 0 exp
qkT"
#$%
&'.
The prefactor 0 and the activation energy q are parameters used to fit experimental data. kT is the temperature in units of energy. If we would rather use the Kelvin (K) as the unit for temperature, the conversion factors between the Kelvin and common units of energy is k = 1.38 x 1023 JK1 = 8.63 x 105 eVK1. We may measure the viscosity of a liquid at several temperatures, and then plot the data on the Arrhenius plot, namely, log vs. kT/1 . The activation energy is found from the slope of the plot, and the prefactor 0 the intercept.
3. A liquid subject to a multiaxial state of stress
Newtons law of viscosity is analogous to Hookes law of elasticity. (I dont know who copied who in this case.) Following an analogous procedure, we may generalize Newtons law to a multiaxial state of stress, ij . Often a liquid is taken to be incompressible; the volumetric strain is typically small compared to the shear strain.
Let v x1,x2,x3( ) be the velocity field. The strain rate is a tensor dij , given by
dij =
12
vixj
+v jxi
"
#$
%
&'
The components of the stress relate to the components of the strain rate as
ij =
vixj
+v jxi
$
%&
'
() +
13 kk ij = 2dij +
13 kk ij .
This is analogous to the generalized Hookes law.
As a special case, under a uniaxial stress , the axial strain rate d / dt relates to the stress as
= 3 d
dt.
The quantity H = 3 defines the viscosity under uniaxial tension.
ES240 Solid Mechanics Fall 2009
11/4/12 Linear Elasticity3
4. Types of deformation
How a material deforms depends on the constitution of the material. We can typically distinguish the following types of behavior:
Elastic strain. Under a load, the solid deforms instantaneously. Upon load removal, the solid recovers its original shape instantaneously. Deformation occurs as a result of bond stretching in crystals or chain straightening in rubbers (crosslinked polymers). Molecules do not change neighbors. Pictorial Representation: The spring. The experimental data is fit to
= /E .
Viscous strain. Under a load, a material deforms indefinitely. Molecules change neighbors. Pictorial Representation: The dashpot. The experimental data is fit to
= H
ddt
Plastic strain. The body does not recover its original shape when the load is removed. Dislocation motion. Crystal rearranges. Atoms change neighbors. Strain is zero when < Y , indefinite when > Y . Pictorial Representation: A sliding block. Static friction.
Elasticplastic model. Spring in series with a frictional block. Isostress. The total strain is the sum of the elastic strain (displacement of the spring) and the plastic strain (displacement of the block).
Thermal strain. The body expands or contracts when the temperature changes. Anharmonic energy well. Pictorial Representation: The spring changes length upon temperature change. Experimental data are often fit to
= T Tref( ) .
5. Linear viscoelasticity
1. Creep test of a viscoelastic rod
A rod of a polymer is held at a constant temperature, stress free, for a long time, so that its length no longer changes with time. The rod is in a state of equilibrium. At time zero, we attach a weight to the rod, and record its elongation as a function of time. Thus, the stress in the rod is a
ES240 Solid Mechanics Fall 2009
11/4/12 Linear Elasticity4
step function of time. The rod is on its way from one equilibrium state to another equilibrium state. The strain is an increasing function of time, with the following characteristics:
1. Unrelaxed strain, U . Instantaneous after we hang the weight to the rod, the rod elongates by a certain amount.
2. Relaxed strain, R . After some time, the molecules reach a new equilibrium configuration, and the strain no long changes with time. This is different from a polymer melt or any liquid.
3. Relaxation time, . The time scale to attain the relaxed strain. The time needed for the rod to change from the old to the new equilibrium state.
Sketch the function ( )t , and mark the above quantities.
To a first approximation, you may fit the record of the history of strain, ( )t , to a function
t( ) = U + R U( ) 1 exp
t
$
%&'
()*
+,

./ .
We all do curve fitting, but some of us are more sophisticated. (We are all in the gutter, but some of us are looking at the stars. Oscar Wilde).
A molecular picture may look like this. When a weight is put on, molecules change configurations by two processes. A fast process occurs right after the weight is put on. A slow process takes place over some time. Of course, a polymer may have more than two processes, and the experimental record of ( )t may not fit to the above formula.
2. Creep compliance
The magnitude of the strain should increase with the weight that we hang to the rod. Say at time zero we load two identical rods, one with weight W, and the other with weight 2W. At any given time, the elongation of the second rod is twice that of the first rod. This linearity holds when the weight is small. We fit this experimental observation by
t( ) = D t( ) ,
ES240 Solid Mechanics Fall 2009
11/4/12 Linear Elasticity5
where is the suddenly applied stress, ( )t is the strain as a function of time, and ( )tD is the compliance as a function of time. We can reinterpret the features of the function ( )t , and denote the unrelaxed compliance by DU, and the relaxed compliance by DR. We may fit the experimental record with a formula:
( ) ( ) !"
#$%
&'(
)*+
,+=tDDDtD URU exp1 .
In general D(t) is a material property and needs to be measured experimentally. We can gain some insight, however, through the following models.
3. Springdashpot models
We next try to interpret the experimental observations. Your basic instinct might tell you to look how molecules pass one another, and try to relate various parameters to all the moving and jamming of the molecules. This approach has been tried as long as the existence of molecules was first appreciated, and has been dubbed as multiscale modeling in recent years. The approach, however, is time consuming, and often not very practical. If you suspend your basic instinct for the time being, you may learn something from simple springdashpot models.
Maxwell model. This model represents a material with a spring in series with a dashpot. Because the two elements, the spring and the dashpot, are subject to the same stress, the model is also known as an isostress model. The total strain is the sum of the elastic and the viscous strain, so that
Hdt
dEdt
d +=
1 .
This is an ODE. For a prescribed history of stress, the ODE can determine the history of strains For example, in the creep test we prescribe the history of stress as a step function:
( )!"#
0. Remember, ( )tD is measured by subject the solid to a step stress.
We next approximate a history of stress by a series of steps of stress:
 At time 0ut = , the stress steps from zero to 0 .
 At time t = u1 , the stress makes an additional step 01
 At time t = u2 , the stress makes yet another step 12
The total strain is the sum of the strains due to all the steps:
t( ) = 0D t u0( ) + 1 0( )D t u1( ) + 2 1( )D t u2( ) .
As an example, consider a rod subject to a stress at time zero. The stress is kept constant fo